11.application of appopolite in adsorption of heavy metals (co and ni) from waste water
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 1, No.2, 2011Application of Appopolite in Adsorption of Heavy Metals (Co and Ni) from Waste Water Rohini Singh1*,Kavita Kulkarni2, A.D.Kulkarni2 1. M.Tech Student, Department of Chemical Engineering, BVDU, Pune, India 2. Associate Professor, BVDU College of Engineering, Pune, India Bharati Vidyapeeth Deemed University, College of Engineering, Pune, 411043, India * E-mail- firstname.lastname@example.org E-mail- email@example.comAbstractThe optimum conditions for adsorption/ion exchange by using a batch method were evaluated by changingvarious parameters such as adsorbent amount, initial pH of the solution, mixing temperature and initial metalions. The influence of the temperature on the ion-exchange/adsorption process was also examined. TheLangmuir and Freundlich adsorption isotherm equations were derived from the basic empirical equations, andused for calculation of ion exchange parameters. Adsorption isotherms of Co2+ & Ni2+ ions could be bestmodelled by the Langmuir equation. The influences of contact time, metal initial concentration, adsorbentdosage concentration, and temperature have been studied. The adsorption efficiencies are found to be contacttime dependent, increasing the contact time in the range of 20–180 min. The sorption equilibrium has attainedbetween 60 and 180 min.Keywords - Adsorption, Freundlich adsorption isotherm, ion exchange, Langmuir equation, sorptionequilibrium1. IntroductionThere are different types of heavy metals which if present in excess quantities in groundwater, river water,lakes, canals, dams and other water bodies leads to serious health disorders and various diseases like irritation ofthe nose, mouth and eyes and it causes headaches, stomachaches, dizziness, vomiting and diarrhoea.The majorsources of heavy metals in the environment include Metal Extraction, Metal Fabrication and Surface Finishing,Paint and Pigments as well as the manufacturing of batteries.2. ZeolitesThe term zeolite was originally coined in the 18th century by a Swedish mineralogist named Cronstedt whoobserved, upon rapidly heating a natural zeolite that the stones began to dance about as the water evaporated.Using the Greek words which mean "stone that boils," he called this material zeolite. A commonly useddescription of a zeolite is a crystalline aluminosilicate with a cage structure. Technically, we speak of a zeoliteas a crystalline hydrated aluminosilicate whose framework structure encloses cavities (or pores) occupied bycations and water molecules, both of which have considerable freedom of movement, permitting ion exchangeand reversible dehydration. This definition places it in the class of materials known as "molecular sieves." [Thepores in dehydrated zeolite are 6 Ångstroms in size, while those of a typical silica gel average about 50 Å, andactivated carbon averages 105 Å.] More than 150 zeolite types have been synthesized and 40 naturally occurringzeolites are known. [The formula of one of the better known zeolites is shown below.] ... Zeolites occur ashydrates, and all members of the family contain at least one silicon atom per aluminum atom.Na-A Na2O · Al2O3 · 2SiO2 · 4.5 H2O 16
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 1, No.2, 20112.1 Natural and Synthetic Formation of ZeolitesZeolites form in nature as a result of the chemical reaction between volcanic glass and saline water.Temperatures favoring the natural reaction range from 27°C to 55°C and the pH are typically between 9 and 10.Nature requires 50 to 50,000 years to complete the reaction. Naturally occurring zeolites are rarely phase-pureand are contaminated to varying degrees by other minerals [e.g. Fe++, SO4-, quartz, other zeolites, andamorphous glass]. For this reason, naturally occurring zeolites are excluded from many important commercialapplications where uniformity and purity are essential. Synthetic zeolites hold some key advantages over theirnatural analogs. The synthetics can, of course, be manufactured in a uniform, phase-pure state. It is also possibleto manufacture desirable zeolite structures which do not appear in nature. Zeolite A is a well-known example.Since the principal raw materials used to manufacture zeolites are silica and alumina, which are among the mostabundant mineral components on earth, the potential to supply zeolites is virtually unlimited. Finally, zeolitemanufacturing processes engineered by man require significantly less time than the 50 to 50,000 yearsprescribed by nature. Zeolites are microporous crystalline hydrated aluminosilicates that can be considered asinorganic polymers built from an infinitely extending three-dimensional network (similar to a honeycomb) oftetrahedral TO4 units, where T is Si or Al, which form interconnected tunnels and cages. Zeolites have beenwidely used in heavy metals adsorption experiments due to their unique physical and chemical properties(crystallinity, thermal stability, well-defined cage structure of molecular size, ion-exchange, etc.). Theadvantage of zeolites over resins, apart from their much lower cost (one ton of the natural zeolite clinoptilolitecosts almost €200), is their ion selectivity. Owing to zeolites structural characteristics and their adsorbentproperties, they have been applied as chemical sieves, water softeners and adsorbents. Zeolites can be easilyregenerated by washing them with acidic solutions (e.g. HCl) and this is one more advantage of them becausethey can be re-used many times without losing their adsorption capability.2.2 Properties of zeolites2.2.1. Ion exchange + + +Zeolites usually contain cations (e.g., Na , K , or NH4 ) after the synthesis. These cations are required tobalance the negative net-charge caused by trivalent aluminum cations which are coordinated tetrahedrally byoxygen anions. By exposing a sodium containing zeolite to a solution containing other cations, the sodium ionscan be exchanged by these other cations provided they are not excluded from the pores due to their size(including the water molecules coordinating the respective cations).2.2.2.MolecularSieveEffect/AdsorptionThe pore sizes of zeolites are determined by their structures and may be varied slightly by ion-exchanging thezeolite. By this process smaller cations can be positioned in windows making them wider. Specific cations mayalso be positioned on other sites than in the windows, thus leading to even larger open windows. The windowsizes determine the accessibility of the zeolite pore system for other (e.g. organic) molecules.2.2.3.AcidityAs already mentioned protonated zeolites have acidic properties. The protons which balance the negative chargeof a zeolite framework are not strongly bound to the framework and are able to move within the pores and reactwith molecules which penetrate into the zeolite pore system. A protonated zeolite thus can act as a Bronstedacid. Furthermore, Lewis acidity can be caused by cations within the pores.2.2.4.CatalysisZeolites make extremely active catalysts.... Steric phenomena are very important in zeolite catalysis, and a newterm, "shape selective catalysis," was coined to describe these effects. Extremely selective reactions can bemade to occur over zeolites [when certain products, reactants or transition states are kept from forming withinthe pores because of size or shape].3. Adsorption isothermThe two isotherms to consider are the Freundlich and Langmuir.3.1 Langmuir isotherm: The Langmuir sorption isotherm is the best known of all isotherms describing sorptionand it has been successfully applied to many sorption processes. Thus, the Langmuir isotherm model is given bythe equation. 17
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 1, No.2, 2011Ce/qe = 1/(Qmax.KL) + Ce/ Qmax ………………. (1)Where,qe = metal concentration on zeolite at equilibrium. (mg of metal ion/g of zeolite)Qmax and KL are the Langmuir constants related to sorption capacity and sorption energy, respectively. Thevalues of Qmax (mg/g) and KL(mg–1) can be determined from the linear plot of Ce/qe vs. Ce.For all cases, the Langmuir model represents a better fit to the experimental data than theFreundlich model.Assumptions:1 .Maximum monolayer coverage (θ=1)2 .Energetically uniform surface.3.No interaction between adsorbate atoms/molecules.4 .The mechanism of adsorption does not change with surface coverage.ra = Kp(1- θ)rd = kI θAt equilibrium, ra= rd θ = Κp/ ( k + Κp) I = Kp/ (1 + Kp) = v / vmWhere, v= volume vm= corrected volume θ = surface coverage (1 - θ) = vacant sites3.2. Freundlich isotherm:The Freundlich isotherm, one of the most widely used mathematical descriptions, usually fits the experimentaldata over a wide range of concentrations. This isotherm is based on adsorption heterogeneous surfaces, theexponential distribution of active sites and their energies and adsorption enthalpy changes logarithmically.This relation is given by:ln qe= ln KF + (1/n).ln Ce……………………(2)where,qe = the amount of metal ions adsorbed per gram of adsorbent at equilibrium (mg/g),Ce is the equilibrium concentration in mg/l,KF = roughly an indicator of the adsorption capacity (mg/g)1/n = a characteristic constant for the adsorption system (g/L).KF and n can be determined from the graph between ln qe vs ln Ce. 18
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 1, No.2, 2011KF = slope and n = intercept.4. ConclusionIn the present study, appopolite, natural zeolite has been successfully used for removal of Co and Ni ions fromthe aqueous model solution. The maximum adsorption of Co has been found at the dosage 5g/l.In between cobalt and nickel cobalt exhibited a higher percentage removal. In addition to this:1. Adsorption of lead, cobalt, and nickel onto appopolite (natural zeolite) has an ion-exchange nature. Threedifferent stages are observed in the ion exchange adsorption of the metals. The process begins with fastadsorption on the appopolite micro crystal surface during the first 20 minutes. Nearly 80% of Copper and 75%of nickel adsorbed during the first stage on the micro crystals surface.2. The ion exchange of metals is directly proportional to pH value of aqueous solutions. Adsorbtion decreases inthe more acidic medium.3. The slight difference between adsorption capacity of the appopolite towards Copper and Cadmium fromsingle and multicomponent solutions may testify to individual sorption centres of the zeolite for each of thesemetals.4. Efficiency of metals removal from solutions by appopolite is inversely proportional to the metalconcentration. The metals from the following order for adsorption efficiency: Pb2+ > Cu2+ > Cd2+ >CO> Ni2+.5. The data obtained from the studies are applied well to the Langmuir isotherm in comparison to the Freundlichisotherm.ReferencesHiraoki katusuki et.al, “Rapid synthesis of Monodispersed α- Fe2O3 Nanoparticles from Fe(NO3)3 solution bymicrowave irradiation”,Journel of the ceramics society of Japan ,112384-387(2004)J.Salado et.al, “Synthesis and magnetic properties of monodispersed Fe2O3 nanoparticles with controlledsizes”,Journal of Non-crystalline solids ,354(2008),5207-5209Brianna R White et.al, “Magnetic ɤ - Fe2O3 nanoparticles coated with poly-L-cysteine for chelation of As(III),Cu(II), Cd(II), Ni(II), Pb(II), and Zn(II)”,Journal of hazardous materials,161(2009),848-853Soamwadee chaianansutcharit et.al, “Synthesis of Fe2O3 nanoparticles in different r,eaction media”CeramicsInternational ,33(2007),697-699Jie chen et.al, “Preparation of Fe3O4 nanoparticles with adjustable morphology”,Journal of alloys andcompounds,(2008) ,Article in press.I.G.Parsons et.al., “Determination of arsenic(III) and arsenic(V) binding to microwave assisted hydrothermalsynthetically prepared Fe3O4,Mn3O4 and MnFe2O4 nanoadsorbents”,Microchemical Journal, 91(2009),100-106.Zhong Jie Zhang et.al, “Hydrothermal synthesis and self assembly of magnetite(Fe3O4) nanoparticles with themagnetic and electrochemical properties”, Journal of crystal growth 310(2008),5453-5457.Pratap Chutia et.al, “Adsorption of As(V) on surfactant modified natural zeolites”Journal of Hazardousmaterials,162(2009),204-211Yu-Ting Zhou et.al, “Removal of Cu2+ from aquous solution by chitosan-coated magnetic nanoparticlesmodified with -ketoglutaric acid”, Journal of colloid and interface science, 330(2009),29-37.Panagiota Stathi et.al, “Physicochemical study of novel organoclays as heavy metal ion adsorbents forenvironmental remediation”,Journal of colloid and interface science, 316(2007),298-309 19
International Journals Call for PaperThe IISTE, a U.S. publisher, is currently hosting the academic journals listed below. The peer review process of the following journalsusually takes LESS THAN 14 business days and IISTE usually publishes a qualified article within 30 days. Authors shouldsend their full paper to the following email address. More information can be found in the IISTE website : www.iiste.orgBusiness, Economics, Finance and Management PAPER SUBMISSION EMAILEuropean Journal of Business and Management EJBM@iiste.orgResearch Journal of Finance and Accounting RJFA@iiste.orgJournal of Economics and Sustainable Development JESD@iiste.orgInformation and Knowledge Management IKM@iiste.orgDeveloping Country Studies DCS@iiste.orgIndustrial Engineering Letters IEL@iiste.orgPhysical Sciences, Mathematics and Chemistry PAPER SUBMISSION EMAILJournal of Natural Sciences Research JNSR@iiste.orgChemistry and Materials Research CMR@iiste.orgMathematical Theory and Modeling MTM@iiste.orgAdvances in Physics Theories and Applications APTA@iiste.orgChemical and Process Engineering Research CPER@iiste.orgEngineering, Technology and Systems PAPER SUBMISSION EMAILComputer Engineering and Intelligent Systems CEIS@iiste.orgInnovative Systems Design and Engineering ISDE@iiste.orgJournal of Energy Technologies and Policy JETP@iiste.orgInformation and Knowledge Management IKM@iiste.orgControl Theory and Informatics CTI@iiste.orgJournal of Information Engineering and Applications JIEA@iiste.orgIndustrial Engineering Letters IEL@iiste.orgNetwork and Complex Systems NCS@iiste.orgEnvironment, Civil, Materials Sciences PAPER SUBMISSION EMAILJournal of Environment and Earth Science JEES@iiste.orgCivil and Environmental Research CER@iiste.orgJournal of Natural Sciences Research JNSR@iiste.orgCivil and Environmental Research CER@iiste.orgLife Science, Food and Medical Sciences PAPER SUBMISSION EMAILJournal of Natural Sciences Research JNSR@iiste.orgJournal of Biology, Agriculture and Healthcare JBAH@iiste.orgFood Science and Quality Management FSQM@iiste.orgChemistry and Materials Research CMR@iiste.orgEducation, and other Social Sciences PAPER SUBMISSION EMAILJournal of Education and Practice JEP@iiste.orgJournal of Law, Policy and Globalization JLPG@iiste.org Global knowledge sharing:New Media and Mass Communication NMMC@iiste.org EBSCO, Index Copernicus, UlrichsJournal of Energy Technologies and Policy JETP@iiste.org Periodicals Directory, JournalTOCS, PKPHistorical Research Letter HRL@iiste.org Open Archives Harvester, Bielefeld Academic Search Engine, ElektronischePublic Policy and Administration Research PPAR@iiste.org Zeitschriftenbibliothek EZB, Open J-Gate,International Affairs and Global Strategy IAGS@iiste.org OCLC WorldCat, Universe Digtial Library ,Research on Humanities and Social Sciences RHSS@iiste.org NewJour, Google Scholar.Developing Country Studies DCS@iiste.org IISTE is member of CrossRef. All journalsArts and Design Studies ADS@iiste.org have high IC Impact Factor Values (ICV).